SYNTHESIS OF NOVEL FUNCTIONALIZED › wp-content › volumes › ... SYNTHESIS OF...
Embed Size (px)
Transcript of SYNTHESIS OF NOVEL FUNCTIONALIZED › wp-content › volumes › ... SYNTHESIS OF...
SYNTHESIS OF NOVEL FUNCTIONALIZED-GRAPHENE/QUANTUM DOTS HYBRID SYSTEM FOR SOLAR CELLS APPLICATION
Saeed Salem Babkair1*, Mohd Taukeer Khan2, Kuldeep Singh3, S K Dhawan4 and Ameer Azam5 1Center of Nanotechnology, Department of Physics, Faculty of Science,
King Abdulaziz University, P.O.Box. 80203. Jeddah 21589 Saudi Arabia 2Lingaya's University, Old Faridabad, Haryana, India, Pin-121002.
3Central Electro Chemical Research Institute (CSIR) Karaikudi-630006, Tamil Nadu, India 4National Physical Laboratory, (CSIR), Dr. K. S. Krishnan Road, New Delhi-110 012, India
5Center of Nanotechnology, King Abdulaziz University, Jeddah 21589, Saudi Arabia *Corresponding author, Email: [email protected]
The present work demonstrates the synthesis of a novel hybrid accepter material containing amino-functionalized graphene oxide and an inorganic semiconducting material, Cadmium Selenide (CdSe). First, amino-functionalized graphene was synthesized and then nanocrystals (NCs) of CdSe were in-situ grown in the functionalized-graphene oxide matrix named f-GCdSe. Structural studies like X-ray diffraction (XRD), Scanning Electron Microscopic (SEM) were employed to investigate the growth of CdSe NCs in graphene matrix. To understand the charge generation and transfer process at the donor/acceptor interface, the absorption, photoluminescence (PL) and transient absorption spectroscopic (TAS) studies have been carried out in poly(3-hexylthiophene) (P3HT)/f-GCdSe thin films. PL quenching in P3HT/f-GCdSe thin film suggests that charge transfer at the donor/acceptor interface. TAS shows higher optical density and longer lived free carriers for P3HT/f- GCdSe thin film. These results suggest that f-GCdSe is an excellent electron acceptor material for OPV devices.
Keywords: Acceptor, functionalized graphene, CdSe nanocomposites, spectroscopy,
Since the past decade a lot of advancement has been accomplished by scientists and engineers in the area of organic photovoltaic (OPV) technology. Recently, double digit power conversion efficiency (PCE) has already been achieved by many groups [1-3]. The main attractive aspect of OPV devices over traditional Si solar cells is their cost-effectiveness as they can be easily manufactured by roll-to-roll processes. In addition, OPV have better performance in low light, can be transparent and colorful, and have greater flexibility and lower weight. The downside of OPV is that their efficiency is still much lower than traditional Silicon solar cells. To make polymer based solar cells an economically interesting alternative, the efficiency of these devices must be increased. The limited efficiency of the OPV is due to the poor carrier mobility , the short exciton diffusion length , the charge trapping , and the mismatch of the absorption spectrum of the active layer and the solar emission . To address these fundamental limitations of polymer solar cells, inorganic NCs
have been blended with organic materials which integrate the benefits of both classes of materials. Various NCs including CdS , CdSe [9,10], CdTe , PbS , ZnO  and TiO2  have been widely studied for hybrid solar cell fabrication. However, the efficiency of organic/inorganic hybrid solar cells reported so far is still less than 5% which is still some distance from the requirement for the next generation of solar cells. A major challenge in developing high-performance organic/inorganic hybrid solar cells is the effective separation of photogenerated electron hole pairs and the transfer of the electrons to the electrode.
Graphene, a monolayer of sp2-hybridized carbon atoms arranged in archetypal two-dimensional lattice, has attracted tremendous attention of OPV scientist and engineers in recent years. The high specific surface area for a large interface, superior electrical mobility up to 10000 cm2V_1s_1, and tunable band gap would make it an excellent electron acceptor in OPV devices . It is of great interest and importance to bind CdSe NCs onto graphene because the combination and interaction between NCs and graphene will lead to multifunctional or even completely new properties in such a nanocomposite [16, 17]. Herein we report the novel in-situ synthesis of CdSe NCs in functionalized graphene matrix, wherein the strategy of in-situ growing CdTe NPs onto P3HT matrix has been adopted . The f-GCdSe nanocomposite shows very fast and dramatically enhanced photoresponse, which makes it an excellent electron acceptor material for OPV devices.
2 SYNTHESIS OF FUNCTIONALIZED- GRAPHENE/CdSe NANOCOMPOISTES
Prior to in-situ synthesis of CdSe nanocrystals in functionalized graphene, aqueous suspension of graphene oxide (GO) has been synthesized from natural graphite powder using modified Hummers method . In a typical process, 3.5 g graphite was charged into a 500 mL beaker and heated for 10 s in a microwave oven to expand the graphite. The resulting graphite was put in 500ml concentrated H2SO4 at 0 ºC with continuous stirring. Then, 21 g of KMnO4 was slowly added and maintained the temperature at 20 °C. The temperature was then elevated to 35 °C, and then 70°C for 2 h with continuous stirring. The flask was then chilled again in the ice bath, and distilled water (ice) was slowly added, maintaining temperature below 70 °C. The mixture was stirred for 1 h and subsequently diluted with 5 L of deionized water. 50 ml of
NSTI-Nanotech 2014, www.nsti.org, ISBN 978-1-4822-5830-1 Vol. 3, 2014 371
Scheme I: Schematic illustration of the in-situ growth of the CdSe NCs in the f-graphene oxide P3HT matrix.
H2O2 (30 wt. %) was added, and vigorous bubbles appeared as the color of the suspension changed from dark brown to yellow. The suspension was centrifuged and washed several times with 10% HCl solution until the pH of the GO dispersion reached 6. The as-synthesized GO dispersion was a paste with a concentration of 1.0 % wt GO. The calculated amount of GO was treated with SOCl2 in DMF followed by octadecylamine ODA at 150°C for 24 hrs to give functionalized graphene. The in-situ synthesized CdSe NCs in graphene was named as f-GCdSe and schematically illustrated in scheme I. In a typical synthesis of f-GCdSe, 100 mg of functionalized graphene was allowed to react with 0.1mmol of cadmium acetate dihydrade at 150 °C in the medium of ODA and the reaction temperature was increased to 300 0C for 2 hrs. The selenium precursor has been prepared by treating 0.2 mmol of selenium powder (Acros Organics) in trioctylphosphine (TOP) (Sigma Aldrich, USA), at 300°C for 30min under nitrogen flow. The Se precursor was then injected in to the functionalized graphene-Cd solution and the mixture was allowed to react for 30 mins at 300°C under nitrogen flow. Growth of CdSe NCs was gets completed when color of the solution turned to dark orange. After the completion of the reaction, the unreacted cadmium acetate and precursor of Selenium were removed by treating nanocomposites with hexane. The reaction mixture was separated by centrifugation and dried in vacuum at 40 °C. Similarly, other compositions of functionalized graphene containing different mole ratios of Cd-acetate were synthesized and are designated as f-GCdSe2 for 0.2 mmol.
3 RESULTS AND DISCUSSION
3.1. Structural Study
The XRD of the f-GO and f-GCdSe nanocomposite are shown in Figure 1. The XRD of nanocomposites powder were
recorded using Rigaku Ultima X-ray diffractometer (40 KV, -K ). The XRD pattern of the f-GO
samples shows a broad peak at 20°. The broad diffraction peak of f-GO can be attributed to two factors: first, the small sheet size (1 μm and below) and, second, a relatively short domain order or turbostratic arrangement of f-GO stacked sheets, each of which broadens the XRD peak . In comparison, XRD data of f-GCdSe shows additional peaks at 2 ~ 25.2°, 42.4°and 49.5° which are attributed to the presence of CdSe NCs in f-GO matrix. These peaks at 2 ~ 25.2°, 42.4°and 49.5° corresponds to the (111), (220) and (311) planes, respectively, of Zinc blend phase of CdSe . The XRD peaks are broadened due to the small size of CdSe NCs. In the XRD spectra of f-GCdSe1, intensity of CdSe peaks at 2 ~ 42.4°and 49.5° are very low attributed to low concentration of CdSe in f- GO. This can also observed from SEM images shown in
~ 19° is almost disappear in f-GCdSe2 due to higher concentration of CdSe in f-GCdSe2 which is also evident in Figure 2(b). The nanoscale morphology is a crucial parameter to understand the effectiveness of the interface for exciton splitting into free charge carriers, and the formation of a percolation network for efficient transport of charge carriers to the electrodes. The surface morphology of the f-GCdSe1 and f-GCdSe2 nanocomposite films have been examined by scanning electron microscopy (SEM) are presented in Figure 2. The SEM micrographs were observed by a field emission scanning electron microscopy (Jeol FESEM-7600F) . It is quite clear that CdSe NCs are evenly distributed within the hybrid system at low CdSe NCs content (Figure 2a) while NCs are massively phase-separated or aggregated from the f- GO matrix at higher NCs content (Figure 2b). An even more drastic contrast between organic and inorganic phases can be observed in f-GCdSe2.
NSTI-Nanotech 2014, www.nsti.org, ISBN 978-1-4822-5830-1 Vol. 3, 2014372
Figure 1 XRD spectra of (a) f-graphene oxide (f-GO), (b) Figure 2